#------------------------------------------------------------------------------
#$Date: 2019-03-05 10:52:05 +0200 (Tue, 05 Mar 2019) $
#$Revision: 213973 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/20/44/7204402.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7204402
loop_
_publ_author_name
'Erwann Jeanneau'
'Nathalie Audebrand'
'Daniel Louër'
_publ_section_title
;
 Synthesis, crystal structure and thermal behaviour of
 CdZrK2(C2O4)4·8H2O
;
_journal_issue                   8
_journal_name_full               'J. Mater. Chem.'
_journal_page_first              2383
_journal_page_last               2389
_journal_paper_doi               10.1039/b202463m
_journal_volume                  12
_journal_year                    2002
_chemical_formula_sum            'C8 H16 Cd K2 O24 Zr'
_chemical_formula_weight         778.03
_space_group_IT_number           82
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  'I -4'
_symmetry_space_group_name_H-M   'I -4'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.000(5)
_cell_angle_beta                 90.000(5)
_cell_angle_gamma                90.000(5)
_cell_formula_units_Z            2
_cell_length_a                   11.216(5)
_cell_length_b                   11.216(5)
_cell_length_c                   8.954(5)
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      34.97
_cell_measurement_theta_min      1.00
_cell_volume                     1126.4(9)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0404
_diffrn_reflns_av_sigmaI/netI    0.0359
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            9787
_diffrn_reflns_theta_full        34.96
_diffrn_reflns_theta_max         34.96
_diffrn_reflns_theta_min         2.57
_exptl_absorpt_coefficient_mu    1.888
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    2.294
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'bipyramidal crystals'
_exptl_crystal_F_000             764
_exptl_crystal_size_max          0.19
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.14
_refine_diff_density_max         0.492
_refine_diff_density_min         -0.464
_refine_diff_density_rms         0.078
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.020(15)
_refine_ls_extinction_coef       0.0109(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.099
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     94
_refine_ls_number_reflns         2482
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.099
_refine_ls_R_factor_all          0.0228
_refine_ls_R_factor_gt           0.0207
_refine_ls_shift/su_max          0.033
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+0.4985P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0459
_refine_ls_wR_factor_ref         0.0468
_reflns_number_gt                2358
_reflns_number_total             2482
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b202463m.txt
_cod_data_source_block           job
_cod_depositor_comments
;
The following automatic conversions were performed:
'_atom_site_symetry_multiplicity' tag replaced with
'_atom_site_symmetry_multiplicity'.

Automatic conversion script
Id: cif_correct_tags 1440 2010-10-19 06:21:57Z saulius 
;
_cod_original_sg_symbol_H-M      I-4
_cod_database_code               7204402
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'y, -x, -z'
'-y, x, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-y+1/2, x+1/2, -z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cd Cd 0.5000 0.5000 0.5000 0.01385(7) Uani 1 4 d S . .
Zr Zr 0.5000 1.0000 0.2500 0.00993(8) Uani 1 4 d S . .
K1 K 0.5000 0.5000 0.0000 0.02395(18) Uani 1 4 d S . .
K2 K 0.5000 1.0000 -0.2500 0.0274(3) Uani 1 4 d S . .
O1 O 0.49630(11) 0.81210(10) 0.18908(15) 0.0209(3) Uani 1 1 d . . .
O2 O 0.48843(12) 0.62189(11) 0.26682(14) 0.0244(3) Uani 1 1 d . . .
C1 C 0.49471(14) 0.72934(13) 0.28841(17) 0.0154(3) Uani 1 1 d . . .
O3 O 0.50183(13) 0.70404(11) 0.55358(14) 0.0232(3) Uani 1 1 d . . .
O4 O 0.50433(11) 0.88886(10) 0.45828(12) 0.0192(2) Uani 1 1 d . . .
C2 C 0.50044(14) 0.77625(14) 0.44890(17) 0.0155(3) Uani 1 1 d . . .
OW1 O 0.70958(15) 0.6456(2) 0.0423(2) 0.0478(5) Uani 1 1 d . . .
OW2 O 0.8587(2) 0.70657(15) 0.2921(2) 0.0472(5) Uani 1 1 d . . .
H11 H 0.751(2) 0.595(2) -0.007(5) 0.050 Uiso 1 1 d D . .
H12 H 0.743(2) 0.654(3) 0.120(3) 0.050 Uiso 1 1 d D . .
H21 H 0.828(3) 0.743(2) 0.367(3) 0.050 Uiso 1 1 d D . .
H22 H 0.911(2) 0.754(3) 0.248(4) 0.050 Uiso 1 1 d D . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zr Zr -2.9673 0.5597 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cd Cd -0.8075 1.2024 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 Cd O3 180.0 ? 4_656 ?
O3 Cd O3 87.587(13) ? . ?
O3 Cd O3 92.413(13) 4_656 . ?
O3 Cd O3 23.68(6) ? 3_566 ?
O3 Cd O3 156.32(6) 4_656 3_566 ?
O3 Cd O3 92.413(13) . 3_566 ?
O3 Cd O3 87.587(13) ? 2_665 ?
O3 Cd O3 92.413(13) 4_656 2_665 ?
O3 Cd O3 156.32(6) . 2_665 ?
O3 Cd O3 92.413(13) 3_566 2_665 ?
O3 Cd O2 45.06(4) ? 3_566 ?
O3 Cd O2 134.94(4) 4_656 3_566 ?
O3 Cd O2 76.88(4) . 3_566 ?
O3 Cd O2 68.68(5) 3_566 3_566 ?
O3 Cd O2 83.35(5) 2_665 3_566 ?
O3 Cd O2 96.65(5) ? 2_665 ?
O3 Cd O2 83.35(5) 4_656 2_665 ?
O3 Cd O2 134.94(4) . 2_665 ?
O3 Cd O2 76.88(4) 3_566 2_665 ?
O3 Cd O2 68.68(5) 2_665 2_665 ?
O2 Cd O2 134.27(4) 3_566 2_665 ?
O3 Cd O2 111.32(5) ? 4_656 ?
O3 Cd O2 68.68(5) 4_656 4_656 ?
O3 Cd O2 83.35(5) . 4_656 ?
O3 Cd O2 134.94(4) 3_566 4_656 ?
O3 Cd O2 76.88(4) 2_665 4_656 ?
O2 Cd O2 66.67(7) 3_566 4_656 ?
O2 Cd O2 134.27(4) 2_665 4_656 ?
O3 Cd O2 103.12(4) ? . ?
O3 Cd O2 76.88(4) 4_656 . ?
O3 Cd O2 68.68(5) . . ?
O3 Cd O2 83.35(5) 3_566 . ?
O3 Cd O2 134.94(4) 2_665 . ?
O2 Cd O2 134.27(4) 3_566 . ?
O2 Cd O2 66.67(7) 2_665 . ?
O2 Cd O2 134.27(4) 4_656 . ?
O3 Cd O2 68.68(5) ? ? ?
O3 Cd O2 111.32(5) 4_656 ? ?
O3 Cd O2 96.65(5) . ? ?
O3 Cd O2 45.06(4) 3_566 ? ?
O3 Cd O2 103.12(4) 2_665 ? ?
O2 Cd O2 113.33(7) 3_566 ? ?
O2 Cd O2 45.73(4) 2_665 ? ?
O2 Cd O2 180.0 4_656 ? ?
O2 Cd O2 45.73(4) . ? ?
O1 Zr O1 93.599(18) . 8_655 ?
O1 Zr O1 93.599(18) . 7_465 ?
O1 Zr O1 150.98(7) 8_655 7_465 ?
O1 Zr O1 150.98(7) . 2_675 ?
O1 Zr O1 93.599(18) 8_655 2_675 ?
O1 Zr O1 93.599(18) 7_465 2_675 ?
O1 Zr O4 138.21(5) . 2_675 ?
O1 Zr O4 79.82(5) 8_655 2_675 ?
O1 Zr O4 76.13(5) 7_465 2_675 ?
O1 Zr O4 70.79(5) 2_675 2_675 ?
O1 Zr O4 76.13(5) . 7_465 ?
O1 Zr O4 138.21(5) 8_655 7_465 ?
O1 Zr O4 70.79(5) 7_465 7_465 ?
O1 Zr O4 79.82(5) 2_675 7_465 ?
O4 Zr O4 133.70(4) 2_675 7_465 ?
O1 Zr O4 79.82(5) . 8_655 ?
O1 Zr O4 70.79(5) 8_655 8_655 ?
O1 Zr O4 138.21(5) 7_465 8_655 ?
O1 Zr O4 76.13(5) 2_675 8_655 ?
O4 Zr O4 133.70(4) 2_675 8_655 ?
O4 Zr O4 67.56(7) 7_465 8_655 ?
O1 Zr O4 70.79(5) . . ?
O1 Zr O4 76.13(5) 8_655 . ?
O1 Zr O4 79.82(5) 7_465 . ?
O1 Zr O4 138.21(5) 2_675 . ?
O4 Zr O4 67.56(7) 2_675 . ?
O4 Zr O4 133.70(4) 7_465 . ?
O4 Zr O4 133.70(4) 8_655 . ?
O2 K1 O2 180.0 ? 4_655 ?
O2 K1 O2 41.27(4) ? . ?
O2 K1 O2 138.73(4) 4_655 . ?
O2 K1 O2 41.27(4) ? 2_665 ?
O2 K1 O2 138.73(4) 4_655 2_665 ?
O2 K1 O2 59.78(6) . 2_665 ?
O2 K1 O2 120.22(6) ? 3_565 ?
O2 K1 O2 59.78(6) 4_655 3_565 ?
O2 K1 O2 138.73(4) . 3_565 ?
O2 K1 O2 138.73(4) 2_665 3_565 ?
O2 K1 OW1 57.02(5) ? . ?
O2 K1 OW1 122.98(5) 4_655 . ?
O2 K1 OW1 69.14(5) . . ?
O2 K1 OW1 97.38(5) 2_665 . ?
O2 K1 OW1 71.54(5) 3_565 . ?
O2 K1 OW1 108.46(5) ? 2_665 ?
O2 K1 OW1 71.54(5) 4_655 2_665 ?
O2 K1 OW1 97.38(5) . 2_665 ?
O2 K1 OW1 69.14(5) 2_665 2_665 ?
O2 K1 OW1 122.98(5) 3_565 2_665 ?
OW1 K1 OW1 164.91(7) . 2_665 ?
O2 K1 OW1 82.62(5) ? 3_565 ?
O2 K1 OW1 97.38(5) 4_655 3_565 ?
O2 K1 OW1 122.98(5) . 3_565 ?
O2 K1 OW1 71.54(5) 2_665 3_565 ?
O2 K1 OW1 69.14(5) 3_565 3_565 ?
OW1 K1 OW1 90.988(10) . 3_565 ?
OW1 K1 OW1 90.988(10) 2_665 3_565 ?
O2 K1 OW1 110.86(5) ? 4_655 ?
O2 K1 OW1 69.14(5) 4_655 4_655 ?
O2 K1 OW1 71.54(5) . 4_655 ?
O2 K1 OW1 122.98(5) 2_665 4_655 ?
O2 K1 OW1 97.38(5) 3_565 4_655 ?
OW1 K1 OW1 90.988(10) . 4_655 ?
OW1 K1 OW1 90.988(10) 2_665 4_655 ?
OW1 K1 OW1 164.91(7) 3_565 4_655 ?
O2 K1 H11 62.4(8) ? . ?
O2 K1 H11 117.6(8) 4_655 . ?
O2 K1 H11 83.5(8) . . ?
O2 K1 H11 98.6(8) 2_665 . ?
O2 K1 H11 60.1(9) 3_565 . ?
OW1 K1 H11 16.5(6) . . ?
OW1 K1 H11 164.6(5) 2_665 . ?
OW1 K1 H11 75.9(5) 3_565 . ?
OW1 K1 H11 103.8(5) 4_655 . ?
OW2 K2 OW2 164.69(8) 4_655 3_575 ?
OW2 K2 OW2 91.017(11) 4_655 5_454 ?
OW2 K2 OW2 91.017(11) 3_575 5_454 ?
OW2 K2 OW2 91.017(10) 4_655 6_664 ?
OW2 K2 OW2 91.017(11) 3_575 6_664 ?
OW2 K2 OW2 164.69(8) 5_454 6_664 ?
OW2 K2 O4 69.67(4) 4_655 1_554 ?
OW2 K2 O4 96.14(5) 3_575 1_554 ?
OW2 K2 O4 118.81(5) 5_454 1_554 ?
OW2 K2 O4 76.03(5) 6_664 1_554 ?
OW2 K2 O4 118.81(5) 4_655 8_655 ?
OW2 K2 O4 76.03(5) 3_575 8_655 ?
OW2 K2 O4 96.14(5) 5_454 8_655 ?
OW2 K2 O4 69.67(4) 6_664 8_655 ?
O4 K2 O4 144.51(4) 1_554 8_655 ?
OW2 K2 O4 96.14(5) 4_655 2_674 ?
OW2 K2 O4 69.67(4) 3_575 2_674 ?
OW2 K2 O4 76.03(5) 5_454 2_674 ?
OW2 K2 O4 118.81(5) 6_664 2_674 ?
O4 K2 O4 51.06(6) 1_554 2_674 ?
O4 K2 O4 144.51(4) 8_655 2_674 ?
OW2 K2 O4 76.03(5) 4_655 7_465 ?
OW2 K2 O4 118.81(5) 3_575 7_465 ?
OW2 K2 O4 69.67(4) 5_454 7_465 ?
OW2 K2 O4 96.14(5) 6_664 7_465 ?
O4 K2 O4 144.51(4) 1_554 7_465 ?
O4 K2 O4 51.06(6) 8_655 7_465 ?
O4 K2 O4 144.51(4) 2_674 7_465 ?
C1 O1 Zr 121.72(11) . . ?
C1 O1 O4 65.93(9) . . ?
Zr O1 O4 55.82(4) . . ?
C1 O1 O4 150.92(11) . 7_465 ?
Zr O1 O4 53.03(4) . 7_465 ?
O4 O1 O4 102.54(6) . 7_465 ?
C1 O1 O4 151.25(11) . 8_655 ?
Zr O1 O4 51.12(4) . 8_655 ?
O4 O1 O4 99.57(6) . 8_655 ?
O4 O1 O4 53.25(5) 7_465 8_655 ?
C1 O1 O1 103.98(12) . 8_655 ?
Zr O1 O1 43.201(9) . 8_655 ?
O4 O1 O1 55.53(5) . 8_655 ?
O4 O1 O1 88.51(4) 7_465 8_655 ?
O4 O1 O1 50.05(4) 8_655 8_655 ?
C1 O2 Cd 113.84(11) . . ?
C1 O2 O3 61.04(9) . . ?
Cd O2 O3 52.88(5) . . ?
C1 O2 O2 167.39(12) . 2_665 ?
Cd O2 O2 56.67(3) . 2_665 ?
O3 O2 O2 109.30(4) . 2_665 ?
C1 O2 K1 128.57(11) . . ?
Cd O2 K1 116.78(6) . . ?
O3 O2 K1 168.38(6) . . ?
O2 O2 K1 60.11(3) 2_665 . ?
C1 O2 O3 113.44(12) . 4_656 ?
Cd O2 O3 49.17(4) . 4_656 ?
O3 O2 O3 71.83(5) . 4_656 ?
O2 O2 O3 67.82(5) 2_665 4_656 ?
K1 O2 O3 105.96(6) . 4_656 ?
C1 O2 OW1 88.44(11) . . ?
Cd O2 OW1 121.96(6) . . ?
O3 O2 OW1 121.27(7) . . ?
O2 O2 OW1 90.54(6) 2_665 . ?
K1 O2 OW1 57.37(5) . . ?
O3 O2 OW1 158.07(6) 4_656 . ?
C1 O2 O3 107.62(11) . 3_566 ?
Cd O2 O3 46.19(3) . 3_566 ?
O3 O2 O3 68.56(5) . 3_566 ?
O2 O2 O3 59.99(5) 2_665 3_566 ?
K1 O2 O3 100.60(5) . 3_566 ?
O3 O2 O3 94.53(6) 4_656 3_566 ?
OW1 O2 O3 76.56(6) . 3_566 ?
C1 O2 OW1 82.25(10) . 4_655 ?
Cd O2 OW1 152.57(6) . 4_655 ?
O3 O2 OW1 135.47(6) . 4_655 ?
O2 O2 OW1 109.86(5) 2_665 4_655 ?
K1 O2 OW1 56.08(5) . 4_655 ?
O3 O2 OW1 104.76(7) 4_656 4_655 ?
OW1 O2 OW1 78.56(5) . 4_655 ?
O3 O2 OW1 152.85(6) 3_566 4_655 ?
O2 C1 O1 127.09(15) . . ?
O2 C1 C2 119.30(13) . . ?
O1 C1 C2 113.61(12) . . ?
C2 O3 Cd 118.98(10) . . ?
C2 O3 O2 60.57(9) . . ?
Cd O3 O2 58.44(4) . . ?
C2 O3 O3 102.44(12) . 4_656 ?
Cd O3 O3 43.794(7) . 4_656 ?
O2 O3 O3 57.90(4) . 4_656 ?
C2 O4 Zr 119.88(10) . . ?
C2 O4 O4 174.33(12) . 2_675 ?
Zr O4 O4 56.22(3) . 2_675 ?
C2 O4 O1 66.49(9) . . ?
Zr O4 O1 53.40(5) . . ?
O4 O4 O1 109.54(4) 2_675 . ?
C2 O4 K2 119.26(10) . 1_556 ?
Zr O4 K2 120.69(6) . 1_556 ?
O4 O4 K2 64.47(3) 2_675 1_556 ?
O1 O4 K2 173.43(5) . 1_556 ?
C2 O4 OW2 85.26(10) . 4_656 ?
Zr O4 OW2 127.55(6) . 4_656 ?
O4 O4 OW2 94.31(6) 2_675 4_656 ?
O1 O4 OW2 125.64(6) . 4_656 ?
K2 O4 OW2 54.27(4) 1_556 4_656 ?
C2 O4 OW2 76.62(9) . 6_665 ?
Zr O4 OW2 151.94(6) . 6_665 ?
O4 O4 OW2 108.67(4) 2_675 6_665 ?
O1 O4 OW2 135.31(6) . 6_665 ?
K2 O4 OW2 51.19(5) 1_556 6_665 ?
OW2 O4 OW2 72.82(5) 4_656 6_665 ?
C2 O4 OW2 135.70(10) . 3_576 ?
Zr O4 OW2 94.49(5) . 3_576 ?
O4 O4 OW2 49.97(4) 2_675 3_576 ?
O1 O4 OW2 137.37(5) . 3_576 ?
K2 O4 OW2 41.37(3) 1_556 3_576 ?
OW2 O4 OW2 95.47(7) 4_656 3_576 ?
OW2 O4 OW2 61.66(4) 6_665 3_576 ?
O3 C2 O4 126.96(15) . . ?
O3 C2 C1 119.07(12) . . ?
O4 C2 C1 113.97(12) . . ?
K1 OW1 O2 53.49(4) . . ?
K1 OW1 OW1 44.506(5) . 3_565 ?
O2 OW1 OW1 84.28(4) . 3_565 ?
K1 OW1 O2 40.14(4) . 2_665 ?
O2 OW1 O2 40.38(4) . 2_665 ?
OW1 OW1 O2 46.49(4) 3_565 2_665 ?
K1 OW1 H11 89.6(18) . . ?
O2 OW1 H11 133.3(19) . . ?
OW1 OW1 H11 49.8(18) 3_565 . ?
O2 OW1 H11 93(2) 2_665 . ?
K1 OW1 H12 124.5(19) . . ?
O2 OW1 H12 79.9(19) . . ?
OW1 OW1 H12 111(2) 3_565 . ?
O2 OW1 H12 85(2) 2_665 . ?
H11 OW1 H12 106(3) . . ?
K2 OW2 OW2 44.492(5) 5_545 7_565 ?
K2 OW2 H21 135.9(17) 5_545 . ?
OW2 OW2 H21 128(2) 7_565 . ?
K2 OW2 H22 93.5(19) 5_545 . ?
OW2 OW2 H22 52.0(18) 7_565 . ?
H21 OW2 H22 109(3) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cd O3 2.3384(16) ? ?
Cd O3 2.3384(16) 4_656 ?
Cd O3 2.3384(16) . ?
Cd O3 2.3384(16) 3_566 ?
Cd O3 2.3384(16) 2_665 ?
Cd O2 2.4990(16) 3_566 ?
Cd O2 2.4990(16) 2_665 ?
Cd O2 2.4990(16) 4_656 ?
Cd O2 2.4990(16) . ?
Cd O2 2.4990(16) ? ?
Zr O1 2.1774(15) . ?
Zr O1 2.1774(15) 8_655 ?
Zr O1 2.1774(15) 7_465 ?
Zr O1 2.1774(15) 2_675 ?
Zr O4 2.2437(14) 2_675 ?
Zr O4 2.2437(14) 7_465 ?
Zr O4 2.2437(14) 8_655 ?
Zr O4 2.2437(14) . ?
K1 O2 2.7556(17) ? ?
K1 O2 2.7556(17) 4_655 ?
K1 O2 2.7556(17) . ?
K1 O2 2.7556(17) 2_665 ?
K1 O2 2.7556(17) 3_565 ?
K1 OW1 2.887(2) . ?
K1 OW1 2.887(2) 2_665 ?
K1 OW1 2.887(2) 3_565 ?
K1 OW1 2.887(2) 4_655 ?
K1 H11 3.01(3) . ?
K2 OW2 2.832(2) 4_655 ?
K2 OW2 2.832(2) 3_575 ?
K2 OW2 2.832(2) 5_454 ?
K2 OW2 2.832(2) 6_664 ?
K2 O4 2.8947(17) 1_554 ?
K2 O4 2.8947(17) 8_655 ?
K2 O4 2.8947(17) 2_674 ?
K2 O4 2.8947(17) 7_465 ?
O1 C1 1.286(2) . ?
O1 O4 2.561(2) . ?
O1 O4 2.726(2) 7_465 ?
O1 O4 2.837(2) 8_655 ?
O1 O1 3.174(2) 8_655 ?
O2 C1 1.2227(19) . ?
O2 O3 2.732(2) . ?
O2 O2 2.746(3) 2_665 ?
O2 O3 3.010(2) 4_656 ?
O2 OW1 3.204(2) . ?
O2 O3 3.219(2) 3_566 ?
O2 OW1 3.300(3) 4_655 ?
C1 C2 1.5317(19) . ?
O3 C2 1.239(2) . ?
O3 O3 3.376(2) 4_656 ?
O4 C2 1.267(2) . ?
O4 O4 2.495(3) 2_675 ?
O4 K2 2.8947(17) 1_556 ?
O4 OW2 3.272(2) 4_656 ?
O4 OW2 3.527(3) 6_665 ?
O4 OW2 4.261(3) 3_576 ?
OW1 OW1 4.118(3) 3_565 ?
OW1 O2 4.239(3) 2_665 ?
OW1 H11 0.86(3) . ?
OW1 H12 0.80(2) . ?
OW2 K2 2.832(2) 5_545 ?
OW2 OW2 4.041(3) 7_565 ?
OW2 H21 0.85(3) . ?
OW2 H22 0.89(3) . ?
